An Acoustics Operations Study for Loblolly Pine (Pinus taeda) Standing Saw Timber with Different Thinning History
There is currently a request from landowners in southeastern USA to provide a nondestructive tool that can differentiate the quality between stands of 25 and 30 years of age subjected to different thinning treatments. A typical site with various thinning regimes was used to vary the wood quality and to determine whether acoustics had the ability to separate for stiffness differences at a given age and local geography. A stand at age 29 with three different spacing (prior thinning) levels was chosen. Three hundred trees (100 per treatment) were randomly selected and acoustically tested for sound velocity using the Time-of-Flight (ToF) method for unthinned, thinned, and twice-thinned stands, respectively. The key finding of the study was that the estimated stiffness of the previously thinned treatments was actually greater than that of the unthinned group, despite having diameters as much as 28% larger. During a forest cruise, knowing that a higher-diameter stand is similar or higher in stiffness could raise the dollar value and harvest priority.
Determining the predictive accuracy of whole tree modulus of elasticity (MOE) of 14-year-old loblolly pine using density and dynamic MOEs estimated by three different acoustic tools
Resonance based acoustic tools for evaluating wood properties have been reported to be more accurate in estimating the expected log MOE than time-of-flight (ToF) ones. However, there is no published study on the variations within different brands on these two major classes of acoustic tools. In this study, models were developed to predict the whole tree static MOE (WMOET) and rupture (WMORT) using log dynamic MOEs estimated by two resonance tools [Director HM200 (EHM200) and FAKOPP resonance log grader (ERLG)], ToF [FAKOPP Microsecond Timer (EFMT)], and density (green density, air-dry density) for a 14-year-old loblolly pine stand from two sites in the southern USA. The log velocity estimated by ToF was 33 and 30% more as compared to the resonance-based tools (Director HM200 and FAKOPP RLG respectively); translating into whole log static MOE (WMOEL) been 11 and 20% lower than those estimated by the resonance (HM200 and RLG respectively), and 90% lower than that estimated by the ToF tools (EFMT). Although the dynamic MOE estimated by ToF tool (EFMT) was higher, its WMOET predictive performance (R2 = 51%) lies between the 39 and 74% for the resonance based tools (HM200 and RGL respectively). This result supports the theory that ToF tools generate dilatational wave, and hence their velocity will be generally higher than resonance tools. The presence of predictive variation within the resonance suggests the need for within tools calibration. The linear relationship between the WMOET vs Etree was stronger than that of WMOET vs EHM200 suggesting that the ToF acoustic tool measurements are not restricted to the outer wood zone for small diameter logs.
Hygroscopic Expansion of some Casting Investments
CREDIT is generally given to Taggart1 for introducing the cast gold inlay to the dental profession. Although he realized that gold shrinks when cooled from molten state to solid state of room temperature, the investment available to him did not supply sufficient compensation. In 1910, Van Horn2 published a paper dealing with a method by which he obtained the compensation by means of wax expansion. The next major research in connection with this problem was the work of Coleman3 at the National Bureau of Standards. He determined the gold shrinkage to be 1.25 per cent and presented a casting technic with compensation values of quantitative nature. The total compensation for the gold shrinkage was obtained by the combination of the setting and thermal expansion of the mold. This procedure is the general practice followed at the present time for compensation. There are some disadvantages to this method. Skinner has indicated the difficulty of obtaining smooth castings and the improper compensation for the casting shrinkage.4 It has been found by Hollenback5 and Scheu6a that castings made at a high temperature are rougher than those made at a low temperature (450° C.), depending upon the great difference in thermal expansion between plaster of Paris and silica, which causes a poor union of the fine particles. This may also result in friability and there may be some warpage due to the differential expansion. A method which provides sufficient compensation at a low mold temperature is the hygroscopic casting technic.b Wilson7 showed that certain plasters expand as much as 0.0044 inch to the inch by taking up moisture from the air. With this information at hand, Scheula, b tested some commercial investment to determine what results the addition of moisture would have. He found6b: (1) All of the casting investments that were tested expanded. (2) The thicker the mix, the greater the expansion. (3) A mix with hot water expanded more than one with cold water. (4) The time at which the mix is placed in the water is of great importance. It was found that if the mix is placed in the water early, it would not expand so much as when placed in a little later. It was also found that if the mix was placed in the water after a certain time, it could not expand to the maximal amount. (5) The temperature of the water in which the mix is placed is important, for two reasons; (a) the temperature of the water controls slightly the expansion of the investment, and (b) water at a temperature of 1000 F. slightly softens the wax pattern so that the fine margins are not marred while expansion is taking place. The mix should remain in the water at least 20 minutes to obtain the full expansion, after which time no further expansion is obtained.